New Vanadium Selenites: Centrosymmetric Ca2(VO2)2(SeO3)3(H2O)2, Sr2(VO2)2(SeO3)3, and Ba(V2O5)(SeO3), and Noncentrosymmetric and Polar A4(VO2)2(SeO3)4(Se2O5) (A = Sr2+ or Pb2+)
Jeongho Yeon; Sang-Hwan Kim; Sau Doan Nguyen; Hana Lee; P. Shiv Halasyamani; Inorganic Chemistry 51 (2012) 609–619; doi:10.1021/ic2021403

data_4327890
_publ_contact_author_address
;
Department of Chemistry
University of Houston
Houston, Texas
77204-5003
USA
;
_publ_contact_author_email       psh@uh.edu
_publ_contact_author_fax         1-713-743-0796
_publ_contact_author_name        'P. Shiv Halasyamani'
_publ_contact_author_phone       1-713-743-3278
_publ_section_title
;
 New Vanadium Selenites: Centrosymmetric Ca2(VO2)2(SeO3)3(H2O)2,
 Sr2(VO2)2(SeO3)3, and Ba(V2O5)(SeO3), and Noncentrosymmetric and Polar
 A4(VO2)2(SeO3)4(Se2O5) (A = Sr2+ or Pb2+)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              609
_journal_page_last               619
_journal_paper_doi               10.1021/ic2021403
_journal_volume                  51
_journal_year                    2012
_chemical_absolute_configuration unk
_chemical_formula_sum            'O21 Se6 Sr4 V2'
_chemical_formula_weight         1262.12
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           43
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'F 2 -2d'
_symmetry_space_group_name_H-M   'F d d 2'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   25.161(3)
_cell_length_b                   12.1579(15)
_cell_length_c                   12.8592(16)
_cell_measurement_reflns_used    6067
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      29.08
_cell_measurement_theta_min      2.44
_cell_volume                     3933.7(8)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 0.939
_diffrn_measurement_device_type  'Siemens area detector diffractometer'
_diffrn_measurement_method       omega_scans
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0305
_diffrn_reflns_av_unetI/netI     0.0281
_diffrn_reflns_limit_h_max       34
_diffrn_reflns_limit_h_min       -34
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            6067
_diffrn_reflns_theta_full        25
_diffrn_reflns_theta_max         29.08
_diffrn_reflns_theta_min         2.44
_exptl_absorpt_coefficient_mu    22.888
_exptl_absorpt_correction_T_max  0.2618
_exptl_absorpt_correction_T_min  0.208
_exptl_absorpt_correction_type   psi-scan
_exptl_absorpt_process_details   'north et al., 1968'
_exptl_crystal_colour            'pale yellow'
_exptl_crystal_density_diffrn    4.262
_exptl_crystal_description       block
_exptl_crystal_F_000             4560
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.08
_refine_diff_density_max         0.506
_refine_diff_density_min         -0.478
_refine_diff_density_rms         0.111
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.001(9)
_refine_ls_extinction_coef       0.000056(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.088
_refine_ls_matrix_type           full
_refine_ls_number_parameters     151
_refine_ls_number_reflns         2384
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.088
_refine_ls_R_factor_all          0.0233
_refine_ls_R_factor_gt           0.022
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0317P)^2^+7.6126P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.058
_refine_ls_wR_factor_ref         0.0583
_reflns_number_gt                1372
_reflns_number_total             1372
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic2021403_si_004_4.cif
_cod_data_source_block           Sr4(VO2)2(SeO3)4(Se2O5)
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Psi scan' changed to
'psi-scan' according to the built-in table from CIF Core dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_database_code               4327890